SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS


 Darren Marcus Hunt
 1 years ago
 Views:
Transcription
1 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS Umar Farooq and Karl Gregory Built Environment and Engineering Department, University of Bolton, United Kingdom ABSTRACT This study deals with the computational modeling of ply by ply failure prediction of filament wound composite tubes under internal burst pressure and external compressive loads with consideration to bending shear. Plates and beams resist transverse load through flexural bending while pressure vessels, pipes, domes, caps and shell like structural composite elements react to the load through membrane forces. Bending stresses are usually neglected in studying behaviour of such elements despite the fact that the bending stresses affect damage modes. Standard failure criteria do not exist for the fibre reinforced composite structural elements hence failure predictions are somewhat unreliable. To consider the flexural shear stresses, methodology of comparative approach involving comparison of failure predictions was adopted. Failure predictions from TsaiHill and TsaiWu criteria were complemented herein with comparison from Hashin s criteria, which utilize such bending stresses. Interaction of the internal pressure and compressive loads were incorporated into the commercially available finite element analysis software ABAQUS TM. To evaluate the effect of loads on deformation and induced changes in tubes, the framework of analysis based on the finite element method provides an exciting capability for analyzing the effects of laminates layup, complicated interaction between the formation of multiple matrixcracks and delamination, orientation and shear effects. Simulation model was developed to use the builtin failure prediction facility of the Hashin criteria. Simple steps were carried out using equations of the other failure criteria to calculate and compare strength parameters for failure predictions. The generated results correlated well and have improved the confidence of accuracy. Simulations can be repeated and extended for similar models subjected to multiple loading. One set of the results consisting of eight unsymmetric plies was selected for presentation herein in the form of legend tables, graphs and contour plots. The study indicates that the approach is useful to predict reliable failure predictions and design improvements for composite wound tubes. Keywords: wound tubes, low velocity impact, finite element simulation, internal pressure, adaptive meshing. 1. INTRODUCTION Lightweight, high stiffness and high strength fibrous composites are being widely used in the construction of pressure vessels such as hollow cylindrical tubes for military and civilian applications. A primary use of wound tube is the fabrication of pressure containment structures such as rocket motor cases, launch tubes, and cold storage vessels. The tube casings are used for burning solid propellants, where both design parameters are important. The solid fuel burns and creates high pressure. This causes large hoop strains and expansion in the diameter of the casing. If this expansion is allowed, the propellant would crack due to increased burning rate build up pressure. Casings made from isotropic materials can reduce the expansion by using very thick casings which is not an acceptable solution. However, filamentwound casings made of composite materials can reduce the expansion due to the orthotropic nature of composites without resorting to large thicknesses. The tubes are built with laminates having several layers with various orientations, the layer orientations are chosen to provide adequate stiffness and strength in the direction of the applied loads, taking into account that the composite material is much stronger and stiffer in the fibre direction. The winding angle determines two parameters: resistance to pressure and resistance to expansion in diameter. From the literature review; it was found that improved computational models in the design and analysis of such tubes are direly needed. Some of the relevant studies conducted in this area are given below: Most of the existing studies of composite cylinders are based on the Lekhnitskii s theory which can be seen in (Lekhnitskii, 1981). Roy and Tsai in (Roy, 1988) proposed a simple and efficient design method for thick composite cylinders for both openended (pipes) and closedended (pressure vessel) cases. Sayman in (Sayman, 005) studied the analysis of multilayered composite cylinders under hygrothermal loading. Xia et al., in (Xia, 001) studied multilayered filament wound composite pipes under internal pressure. Xia et al., in (Xia, 00) presented an exact solution for multilayered filament wound composite pipes with resin core under pure bending. Parnas and Katırcı in (Parnas, 004) discussed the design of fibrous pressure vessels under various loading conditions based on thickwalled, multilayered, filament wound cylindrical shell. Roy and Massard in (Roy, 199) studied the design of thick multilayered composite spherical pressure vessels based on 3D linear elastic solution using TsaiWu failure criterion discovering that hybrid spheres increased the burst pressure. Adali et al., in (Adali, 1995) presented another method on the optimization of multilayered pressure vessels using 3D interactive TsaiWu failure 75
2 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. criterion to predict the maximum burst pressure. Sun et al., in (Sun, 1999) calculated the stresses and the burst pressure of filament wound solidrocket motor cases using maximum stress failure criteria and stiffnessdegradation model. The effect of surface cracks on strength was investigated theoretically and experimentally for glass/epoxy filament wound pipes, by Tarakçioğlu et al., in (Tarakçioğlu, 000). Mirza et al., in (Mirza, 001) investigated the composite vessels under concentrated moments applied at discrete lug positions using the finite element method. Experimental and computational studies were carried out by Aziz et al., in (Aziz, 008) to predict failure of the composite tubes. Most of the existing studies in the literature are experimental, time consuming, expensive and lack in reliable failure predictions. A simulation model consisting of ply by ply prediction of strength parameters efficiently is needed. Current study complements the existing research and focuses on developing simulation model considering coupling effects on progressive failure prediction of cylindrical wound tubes to improve predictions for reliable designs.. DAMAGE AND PROGRESSIVE FAILURE MODES AND HASHIN S FAILURE CRITERIA Damage modes may occur in matrix tensile cracking, matrix compressive/shear failure, ply separation (delamination) and fibre breakage (tensile or compressive). Interalamina (ply) failure can occur by fibre breakage, cracking of matrix, and debonding between fibre and matrix. Interlaminer failure occurs by delamination. Fibre breaking occurs for all systems where fibre fracture strain is less than matrix fracture strain. Fibre breakage manifests itself as deviation from linear stressstrain or loaddeflection curve. Composites with brittle matrix and highstraintofailure fibre fail by matrix cracking of the matrix. Matrix cracking is promoted by the triaxial stresses generated by constraint fibres. Matrix cracking does not have much effect on loaddeformation or stressstrain curve since the strength contribution of the matrix is small compared to the fibre. Fibre breakage and matrix cracking result in total failure. Weak interfaces between fibre and matrix lead to debonding. In a longitudinal tensile test of a unidirectional composite no evident debonding is apparent in loaddeflection curve. Failure surfaces exhibiting fibre pullout is the usual evidence for debonding. Debonding is promoted by different Poisson ratios between fibre and matrix which lead to tensile stresses across the fibrematrix interface. Under these conditions, all six stress components are generally necessary to characterize and discriminate among the various possible failure modes..1 Fibre failure modes The fibre tensile mode is assumed to depend only on the axial stress, and the fibre tensile failure is predicted when σ 1 l S1 = 1 l Where S 1 is the axial tensile strength? This criterion is applicable when σ 1 is positive, and is used to predict a failure mode characterized by fibre breakage. When fibre failure in tension is predicted in a layer, the load carrying capacity of that layer is completely eliminated. The axial modulus E a, the transverse modulus E t, the shear modulus G a and the transverse shear modulus G t are all reduced to zero. When σ 1 is compressive it is assumed that failure is characterized by fibre buckling and is only depended upon σ 1. The compressive fibre mode failure criterion is governed by the maximum stress criterion σ 1 c S1 = 1 c S 1 Where is the axial compressive strength of the ply. For compressive fibre failure, the layer is assumed to carry a residual axial load, while the transverse load carrying capacity is reduced to zero.. Matrix failure modes Matrix failure mode is characterised by cracks running parallel to the fibres. Failure is described as being tensile or compressive, depending upon the sign of the quantity (σ + σ 3 ). Both matrix mode failure criteria assume quadratic interactions between the thickness, (both inplane, σ and through the thickness, σ 3 ), the maximum shear in the transverse plane, and the maximum axial shear. When (σ + σ 3 ) is positive, the tensile mode criterion is used. This criterion is given by F t σ + σ 3 = t S t S τ 3 σ σ 3 + S 3 + τ 1 + S τ 31 1 = 1 Where, S3 and S 1 are the transverse tensile, transverse shear and axial strengths, respectively. For (σ + σ 3 ) negative, the compressive failure criterion is given by F c σ σ 3 = S 3 + τ 3 + τ 1 + S τ 31 = 1 This is a simple quadratic interaction between maximum transverse stress and axial shear stress. Failure predicted by the criterion is referred to as compressive/shear failure. No stiffness reduction is assumed after matrix failure occurred. This is because transverse matrix cracks alone usually do not have significant effect on the laminate stiffness. 1 (1) () (3) (4) 76
3 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved..3 Delamination modes The first possible failure occurs when matrix cracking leads to decrease in the interlaminar strength as a result further loading and deformation causes delamination. Varying the angle between two layers affects the extent of delaminated areas. Maximum delaminated area is observed for laminates with an orientation angle between two adjacent layers being 90 o. Thin laminates showed regular damage pattern with less delaminated area for all types of separation of the bottommost ply from the rest of the laminate. Thicker laminates also shows an increased delaminated area. All the simulated tests show a difference in delaminated area by varying the orientation angle there is no significant effect on the delaminated area. The delamination crack runs in the resinrich area between plies with different fibre orientation. It has been observed that delamination only occurs in the presence of matrix cracks. Taking this into consideration, the initiation of the delamination mode is determined by scaling the matrix damage functions to higher level of stresses. For (σ + σ 3 ) positive, the tensile shear delamination mode is given by S = 1 (5) F t For (σ + σ 3 ) negative, the compressive/shear delamination mode is given by analytical prediction for the numerical data for the delamination area. When delamination is predicted, the transverse modulus, the axial and transverse shear moduli are reduced to zero in the layer with matrix damage. However, the layer axial modulus is unchanged. The criteria can be extended to 3D problems..4 Hashin s failure criteria (Hashin, 1980) The failure modes included in Hashin s criteria are as follows: Tensile fibre failure for σ 11 0 Compressive fibre failure for σ 11 < 0 Tensile matrix failure for σ + σ 33 > 0 (7) S = 1 (6) F t Where F t and F c are damage functions and S is used as scale factor which can be determined from fitting the Compressive matrix failure for σ + σ 33 < 0 (8) ( σ + σ33 ) σ1 σ 13 Y C σ + σ σ σ σ > = S3 YC 4S3 S3 S1 1 failure 1 no failure (9) Interlaminar tensile failure for σ 33 > 0 σ 1 failure 33 = > Z T 1 no failure Interlaminar compression failure for σ 33 < 0 σ 1 failure 33 = > Z C 1 no failure (10) (11) Where σ ij denote the stress components and the tensile and compressive allowable strengths for lamina are denoted by subscripts T and C, respectively. X T, Y T, Z T denotes the allowable tensile strengths in three respective material directions. Similarly, X C, Y C, Z C denotes the allowable tensile strengths in three respective material directions. Further, S 1, S 13 and S 3 denote allowable shear strengths in the respective principal material directions. A shortcoming of TsaiHill and TsaiWu criteria is that they do not explicitly differentiate matrix failure from fibre failure. Hashin s criterion decomposes into separate fibre and matrix failure modes. It also distinguishes tensile states from compressive states, which separate criterion taken for each. This then involves more terms than just those in TsaiWu; several assumptions were used to bring the parameter count down to a manageable level of the six properties. Hashin developed a set of interactive failure criteria in which distinct failure modes are modelled and defined a general failure criterion in terms of the stress invariants. The five stress invariants (I 1, I, I 3, I 4, and I 5 ) are: I I I I I = σ = σ = σ = σ = σ 11, 1 + σ + σ + σ σ , + σ, + σ 33 σ 3 13, + σ 1 σ 13 σ 3. (1) 77
4 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. The I 5 invariant does not appear in the criterion because only linear and quadratic terms are retained in this polynomial. To identify distinct failure modes, Hashin argued that failure is produced by the normal and shear stresses acting on the failure plane. For failure parallel to the ply, the failure plane is the 3, acted on by stresses σ 11, σ 1, and σ 13. The perpendicular stresses (σ, σ 3, and σ 33 ) do not contribute to parallel failure. Reviewing the literature for existing failure theories the set of criteria Hashin was also selected for this study. For delamination prediction Hashin s failure criteria satisfies the requirements for effective use of transverse shear stresses in addition to membrane failures. 3. COMPUTATIONAL PROCEDURE FOR STRESSES AND FAILURE PREDICTIONS Every material has certain strength, expressed in terms of stress or strain, beyond which it fractures or fails. An object is regarded failed when it can no longer support the loads acting on it or when the component can no longer fulfil the function for which it was designed. Such failures include excessive deflection as seen when a laminate buckles, or even just matrix cracking. The latter could constitute failure for a container because any contents would be able to leak through the matrix cracks in the container's walls. Failure theories for isotropic materials are independent of the direction and are characterized by yield strength. A large number of such criteria exist but no one criterion being universally satisfactory for composites. Failure predictions of composites start by considering a single ply before moving on to laminates. The laminate to be a regular array of parallel continuous fibres perfectly bonded to the matrix have five basic modes of failure of such a ply: longitudinal tensile or compressive, transverse tensile or compressive, or shear. Each of these modes would involve detailed failure mechanisms associated with fibre, matrix or interface failure. First step is to calculate the stresses/strains in the material principal directions. This can be done by transformation of stresses from the global coordinates to local material coordinates of the ply. The constitutive equations are used to calculate the stresses in each ply when the values of the loads acting on the laminate are known. A flowchart for the procedure of stresses and strains in individual ply owing to external loads used to streamline calculations is shown below: Flowchart1. Flowchart for laminate stress analysis (Agarwal, 006). 78
5 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. These stresses and strains can be used to predict the load at which failure initiates, first lamina fails, compared with the corresponding allowable values. Flowchart. Flowchart for laminate strength analysis (Agarwal, 006). The determination of the ultimate failure of laminate requires an iterative procedure taking into account the damage progression in the various plies. The computational procedure for the multiple ply failure approach for the case of a symmetric laminate under inplane loading is illustrated by the flowchart and consists of the following steps: The load required to produce first ply failure is determined from the lamina stresses using a selected failure criterion. The lamina stresses are obtained as a function of the loading and are referred first to the laminate coordinates and then transformed to the lamina coordinates; The failed lamina or laminas are replaced with laminas of reduced stiffness. These usually are the matrixdominated stiffness, the stiffness reduction factors can be selected based on analysis as completely (ply 79
6 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. discount method). New laminate stiffness matrices are then calculated; Lamina stresses are recalculated and checked against the selected failure criterion to verify that the undamaged laminas do not fail immediately under their increased share of stress following the first ply failure; The load is increased until the next ply failure occurs and steps 1,, and 3 above are repeated; and When the remaining undamaged laminas, at any stage of the progressive ply failures, cannot sustain the stresses, ultimate failure of the laminate occurs. Multidirectional laminate is initiated in the layer (or layers) with the highest stress normal to the fibres. Failure initiation takes the form of distributed microcracks with coalesce into micro cracks in the case of a unidirectional lamina under transverse tension while macrocracking extends across the thickness of the layer constitutes. 5. RESULTS AND DISCUSSIONS Simulation selected for presentation are from a small size specimen tube of 1000 mm long, 00 mm radius, and mm thick consisting of eight nonsymmetric ply as shown in Figure1. Specimen properties assigned to the model are of fabric code IM7/855 given in Table1. Configuration of 8ply nonsymmetric layup [45/0/ 45/90/45/0/45/90] with 0.% strain allowance chosen for discussion herein. The chosen layup provides different laminate stiffness for in the other configurations, but delamination remains confined to the [0 0 /90 0 ] interfaces. The tube was fixed at the one end and subjected to a range of compressive loads from 100 kn up to 500 kn along with a constant internal pressure of MPa as shown in Figure4. Table1. Material properties used in the analysis. Property IM7/855 Tensile modulus (E 1 ) GPa 150 Tensile modulus (E ) Gpa 15 Tensile modulus (E 3 ) Gpa 15 Inplane shear modulus (G 1 ) Gpa 5.70 Inplane shear modulus (G 13 ) Gpa 5.70 Inplane shear modulus (G 3 ) Gpa 7.6 Poisons ratio (ν 1 ) 0.33 Poisons ratio (ν 13 ) Poisons ratio (ν 3 ) Ultimate tensile strength GPa 1500 Ultimate compressive strength GPa 1500 Ultimate tensile lateral strength GPa 40 Ultimate compressive lateral GPa 46 strength Ultimate shear strength GPa 68 Figure1. Tube consisting of 8 plies. Figure. Tube under internal and external compressive loads. Figure3. Meshed tube consisting of S 4 shell elements with fine meshes. The tube was meshed with course elements first but automatic adaptive meshing facility was utilized to finely mesh the tube where load intensity is higher. First, simulations were carried out in ABAQUS TM to compute stresses and strains without using builtin Hashin failure criteria. Simulations were performed with incremental load addition until complete failure was reached. Then, simulations were repeated with Hashin s failure criteria. Comparison of plybyply legend 80
7 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. Tables and simulated contour plots from Maximum Strain theory for allowable strains and Hashin s failure theory for strength ratios are shown in Figures 3, 11 below. Failure for all the plies was demonstrated by the simulation as expected under the coupled loads. Simulations were also performed to observe variation of strain energy as shown in Graph 1 and total energy shown in Graph. The graphical variation of strain and total energy are acceptable and according to the expectations which validated the models. Computer generated inplane normal and shear stresses were used to calculate strength ratios from the standard TsaiHill and TsaiWu criteria as shown in Table. Finally, computed and simulated values for failure theories were compared in Graph3. The graph demonstrates that TsaiHill and TsaiWu predicts the similar failure pattern from ply 1 to ply 8 as bending stresses are ignored in these criteria. However, graph line for Hashin s criteria depicts a significant difference in ply 7 and 8. As Hashin criteria regards bending stress acting on the these bottom plies. This further confirms that the bending stresses could cause premature failure and should not be neglected. The results show that strength parameters correlate changes of material properties according to loading variations. Calculated values were compared against the given strength parameters and failure were found as expected. Simulated legend Tables and contour plots for comparison of Max strain and hashin failure criteria Figure4. Comparison of legend table and contour plots for ply 1. Figure5. Comparison of legend table and contour plots for ply. Figure6. Comparison of legend table and contour plots for ply 3. 81
8 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. Figure7. Comparison of legend table and contour plots for ply 4. Figure8. Comparison of legend table and contour plots for ply 5. Figure9. Comparison of legend table and contour plots for ply 6. Figure10. Comparison of legend table and contour plots for ply 7. 8
9 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. Figure11. Comparison of legend table and contour plots for ply 8. Time variation of strain and total energies is shown in the form graphs Graph1. Strain energy (kj) absorbed by the specimen under load. 83
10 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. Graph. Total energy (kj) wavy variation under static load. Table. Computed inplane stresses and strength ratios. Calculation of strength ratio of TsaiWu and TaiHill criteria (Agarwall, 006) Ply No. σ 11 σ σ 1 Strength ratios MPa TsaiWu TsaiHill Graph3. Comparison of strength ratios of the failure criteria. 84
11 VOL. 5, NO. 4, APRIL 010 ISSN Asian Research Publishing Network (ARPN). All rights reserved. 5. CONCLUSIONS In this study progressive failure analysis simulation model was developed for a general laminated tube utilising shear stresses. Results for a special case from 8ply model were illustrated in legend tables, contour plots, tabular and graphical forms. Comparison of standard failure theories was made to predict reliable failures. Results show that for a relatively small range of bottom plies strength ratios for Hashin s criteria are considerably high. This confirms that bending shear has significant effect on failure prediction and could cause failure well below the prediction from the other criteria which neglect the coupling effects. The analysis methodology has been carried out by assuming that the laminate is composed of identical plies. The analysis can be modified easily if the laminate differs in properties and thickness. Simulations include validation of elastic solution from strain and total energies to analyze the burst pressure when standard values are not available for comparison. The burst pressure varies at higher loads when strength has already decreased. Based on the results it may be further concluded that the tested case is unsafe under these loading conditions. REFERENCES Hashin Z Failure Criteria for Unidirectional Fibre Composites. ASME Journal of Applied Mechanics. 47(): S.G. Lekhnitskii Theory of elasticity of an anisotropic body, Mir Publishers, Moscow. A.K. Roy and S.W. Tsai Design of thick composite cylinders. J Press Vessel Technol. 110: View Record in Scopus Cited By in Scopus (8). M. Xia, H. Takayanagi and K. Kemmochi Analysis of multilayered filamentwound composite pipes under internal pressure. Compos Struct. 53: L. Parnas and N. Katırcı. 00. Design of fibrereinforced composite pressure vessels under various loading conditions. Comp Struct. 58: M. Xia, H. Takayanagi and K. Kemmochi. 00. Bending behavior of filamentwound fibre reinforced sandwich pipes. Comp Struct. 56: O. Sayman Analysis of multilayered composite cylinders under hygrothermal loading. Composites Part A. 36: T.K. Hwang, C.S. Hong and C.G. Kim Size effect on the fibre strength of composite pressure vessels. Compos Struct. 59: H. Hahn and S. W. Tsai Nonlinear elastic behavior of unidirectional composite laminate. J. Compos. Mater. 7: ABAQUS/Standard User s Manual, Version 6.5, ABAQUS, Inc., Providence, RI. D. Agarwal Bhagwan, Lawrance J. Brouton and K. Chandrashekkara Analysis and Performance of Fibre Composites. 3 rd Ed. JohnWiley and Sons, Inc. Hoboken, New Jersy, USA. Aziz Onder, Onur Sayman, Tolga Dogan and Necmettin Tarakcioglu Burst failure of composite pressure vessels. Comp. Struct. 49: A.K. Roy and T.N. Massard A design study of multilayered composite spherical pressure vessels. J Reinf Plast Compos. 7: S. Adali and V.E. Verijenko et al., Optimization of multilayered composite pressure vessels using exact solution. Compos Press Vessels Ind PVPV30. pp ASME. Herakovich C T Mechanics of Fibrous Composites. John Wiley and Sons, New York. X.K. Sun, S.Y. Du and G.D. Wang Bursting problem of filament wound composite pressure vessels. Int. J Press Vessels Piping. 76: S. Mirza A. Bryan and M. Noori, Fibrereinforced composite cylindrical vessel with lugs. Compos Struct. 53:
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationINSTITUTE OF AERONAUTICAL ENGINEERING (Autonomous) Dundigal, Hyderabad
INSTITUTE OF AERONAUTICAL ENGINEERING (Autonomous) Dundigal, Hyderabad 00 04 CIVIL ENGINEERING QUESTION BANK Course Name : STRENGTH OF MATERIALS II Course Code : A404 Class : II B. Tech II Semester Section
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationStress Analysis of Radial and Non Radial Nozzle Connections in Ellipsoidal Head Pressure Vessel
Journal of Mechanical Engineering Vol. 10, No. 1, 6783, 2013 Stress Analysis of Radial and Non Radial Nozzle Connections in Ellipsoidal Head Pressure Vessel Haszeme Abu Kasim 1, a Professor Dr. Ir. Wahyu
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationWrinkling Analysis of A Kapton Square Membrane under Tensile Loading
44th AIAA/ASME/ASCE/AHS Structures, Structural Dynamics, and Materials Confere 710 April 2003, Norfolk, Virginia AIAA 20031985 Wrinkling Analysis of A Kapton Square Membrane under Tensile Loading Xiaofeng
More informationMalaysia Phone: ; Fax:
International Conference on Mechanical Engineering Research (ICMER013), 13 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia
More informationCRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES
S. Kakay et al. Int. J. Comp. Meth. and Exp. Meas. Vol. 5 No. (017) 116 14 CRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES SAMDAR KAKAY DANIEL BÅRDSEN
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationLap splice length and details of column longitudinal reinforcement at plastic hinge region
Lap length and details of column longitudinal reinforcement at plastic hinge region HongGun Park 1) and ChulGoo Kim 2) 1), 2 Department of Architecture and Architectural Engineering, Seoul National University,
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationAnalysis of composite hydrogen storage cylinders subjected to localized flame impingements
Available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/he Analysis of composite hydrogen storage cylinders subjected to localized flame impingements J. Hu a, J. Chen a, S. Sundararaman
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationChapter 1  Introduction
Chapter 1  Introduction 1.1 Aft pressure bulkhead On a large transport aircraft, the pressurized cabin is closed at the aft end by a domeshaped pressure bulkhead as is shown in Fig. 1.1. In general,
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationStudying Decreased Methods of Stress Concentration around Holes and Openings of Plate and Shell Structures Body
International Research Journal of Applied and Basic Sciences 01 Available online at www.irjabs.com ISSN 5188X / Vol, 5 (8): 10081015 Science Explorer Publications Studying Decreased Methods of Stress
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationCentrifuge Shaking Table Tests and FEM Analyses of RC Pile Foundation and Underground Structure
Centrifuge Shaking Table s and FEM Analyses of RC Pile Foundation and Underground Structure Kenji Yonezawa Obayashi Corporation, Tokyo, Japan. Takuya Anabuki Obayashi Corporation, Tokyo, Japan. Shunichi
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationShear Behaviour of Fin Plates to Tubular Columns at Ambient and Elevated Temperatures
Shear Behaviour of Fin Plates to Tubular Columns at Ambient and Elevated Temperatures Mark Jones Research Student, University of Manchester, UK Dr. Yong Wang Reader, University of Manchester, UK Presentation
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information